# CSWIP 3.1: Question with Answer and Explanation – Part 3

## CSWIP 3.1 QUESTION AND ANSWER SERIES

(145mb) Books & Chapter wise Questions (General Paper + Technical Paper) and Answers. Examination notes on Practical Examination of Plate/Pipe CSWIP 3.1 Learning Presentation

\$72.00

CSWIP 3.1: Question with Answer and Explanation – Part 1

CSWIP 3.1: Question with Answer and Explanation – Part 2

CSWIP 3.1: Question with Answer and Explanation – Part 3

CSWIP 3.1: Question with Answer and Explanation – Part 4

CSWIP 3.1: Question with Answer and Explanation – Part 5

CSWIP 3.1: Question with Answer and Explanation – Part 6

CSWIP 3.1: Question with Answer and Explanation – Part 7

CSWIP 3.1: Question with Answer and Explanation – Part 8

CSWIP 3.1: Question with Answer and Explanation – Part 9

CSWIP 3.1: Question with Answer and Explanation – Part 10

CSWIP 3.1: Question with Answer and Explanation – Part 11

CSWIP 3.1: Question with Answer and Explanation – Part 12

CSWIP 3.1: Question with Answer and Explanation – Part 13

CSWIP 3.1: Question with Answer and Explanation – Part 14

CSWIP 3.1: Question with Answer and Explanation – Part 15

CSWIP 3.1: Question with Answer and Explanation – Part 16

CSWIP 3.1: Question with Answer and Explanation – Part 17

CSWIP 3.1: Question with Answer and Explanation – Part 18

CSWIP 3.1: Question with Answer and Explanation – Part 19

CSWIP 3.1: Question with Answer and Explanation – Part 20

1) In a welding procedure transverse joint tensile test the following observations were made. The specimen CSA was recorded as 25mm x 12mm and the maximum load applied was recorded as 150kN. What is the UTS?

• Transverse tensile test:
• CSA: cross section area
• UTS: ultimate tensile strength ( N/mm2; p.s.i; Mpa )
• UTS = (150×1000)/(25×12) = 500N/mm2
• Pls take note for unit of value.

2) In welder qualification testing of 10mm plates, 2 root and 2 face bends were test … what course of action would you follow?

• Bend test: To determine the soundness of the weld zone. Bend testing can also be used to give an assessment of weld zone ductility. There are three ways to perform a bend test: Face bend, root bend & side bend (Generally for materials above 12mm thickness).
• But this question is for Welder.

3) In an all weld tensile test, the original specimen gauge length was 50mm, and after the test the increased gauge length was 60mm, what is the elongation percentage?

E= (60-50)*100/50 = 20%. So, righ answer is “b”.

4) Some codes require the excess weld metal (weld cap) on cross weld joint tensile specimens to be flush, this is because:

Note that the stress raiser at the toe of the weld cap will make incorrect stress result.

5) When transverse tensile testing a welded joint the excess weld metal is often removed. This action is done to:

see previous question!

6) In welder qualification testing of 20mm plates, why are side bends used instead of root and face bends:

Bend test: To determine the soundness of the weld zone. Bend testing can also be used to give an assessment of weld zone ductility.

Side bend tests are normally carried out on welds over 12mm in thickness.

When make the “Side bend”, 3 area as: root, face & side will be tested. That tests test the full section thickness. So, it gives more accurate indications.

Specimens and testing for bend testing for butt joints shall be in accordance with EN 910.
For thicknesses < 12 mm two root and two face bend test specimens shall be tested. For thicknesses 12 mm four side bend specimens are recommended instead of root and face bend tests.

7) Mechanical tests are divided into two areas, identify these from the list below:

Quantitative Tests: For measuring a ‘quantity’ ( a mechanical property )

Qualitative Tests: For assessing joint ‘quality’ (good fusion & free from defects)

The following mechanical tests have units and are termed quantitative tests to measure Mechanical Properties:

• Tensile tests (Transverse Welded Joint, All Weld Metal)
• Toughness testing (Charpy, Izod, CTOD)
• Hardness tests (Brinell, Rockwell, Vickers)

The following mechanical tests have no units and are termed qualitative tests for assessing joint quality:

• Macro testing
• Bend testing
• Fillet weld fracture testing
• Butt weld nick-break testing

8) When examining a completed bend test, the angle of the bend was found to be 175o. The testing specification calls for the sample to have been formed through 180o.

9) Charpy testing is carried out on a welding procedure test plate because?

Some question we need use “exclusion method”.

Charpy testing:

a) It gives an indication of the through thickness ductility (in the Z direction):  this for STRA not Charpy impact test.

c) It gives an indication of the materials elongation properties

d)  It gives a quick indication of the weld quality for welder qualification tests: welder qualification test don’t require Chapry impact test.

b) The impact test results can be used to verify that the material has not been adversely affected by the heat of the welding: this is correct answer.

10) Charpy impact tests show a 50% rough torn surface and a 50% flat crystalline surface after the completed test, this would indicate which type of failure?

Charpy impact test: These tests show that metals can be classified as being either ‘brittle’ or ‘ductile’. A brittle metal will absorb a small amount of energy when impact tested, a tough ductile metal a large amount of energy.

Some steels may show transition characteristics in their failure mode from ductile to brittle gradually as temperature is decreased, which is given in Figure-4 schematically. In this case different approaches may be used in determining transition temperature but the average energy concept is the most popular one. Determination of transition temperature can also be done by examining the fracture surfaces of specimens tested at different temperatures. For example the temperature, at which the fracture surface consists 50 percent cleavage (crystalline) and 50 percent ductile (fibrous) types of fracture, is called fracture appearance transition temperature (FATT). Another common criterion is to determine the transition temperature on the basis of an arbitrary energy absorbed.